{'fraction_non_alphanumeric': 0.021870286576168928, 'fraction_numerical': 0.003959276018099547, 'mean_word_length': 5.0697940503432495, 'pattern_counts': {'":': 0, '<': 0, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Continuous Multilayered Carbon Nanotube Yarns

2010 WILEY-VCH Verlag Gm Carbon nanotubes (CNTs) have ultrahigh strength, high electrical conductivities, high thermal conductivities, electric field emissions, gas sensitivities, and other functional properties. These outstandingmechanical, physical, andmultifunctional properties of CNTs, in combination with their unique 1D nanostructures with high specific areas, allow for a wide range of potential applications such as structural fibers, composites, multifunctional fabrics, and devices. The fabrication of CNTs into a continuous multifunctional CNT yarn is an important step towards these macroscopic applications. Several processes are under development to fabricate macroscopic CNT fibers, including wet spinning of CNTs from polymer dispersions or acid dispersions, dry spinning from aligned CNT matrices, and direct spinning from chemical vapor deposition (CVD) reactions. While the development of a continuous and weavable pure CNT yarn remains a major challenge in the fabrications, CNT yarns so far obtained from the different processes are monolithic in structure, although a hollow yarn was demonstrated from a wet drawing process. One the other hand, CNT sheets or films have been fabricated by drying CNT dispersions, drawing [19,20] or infiltrating of CNT arrays, and by CVD spinning. These 2D CNT assemblies have demonstrated applications as catalyst supports, molecular sieves, infiltrators, conductors, electromagnetic shields, capacitors, and artificial tissues. If CNTs can be made into continuous yarns with a layered structure, they will combine the weavable property of fibers and the structural characteristic of films and can be adopted for numerous applications. In the present work, we report the fabrication of a novel continuous yarn of CNTs with a multiple-layer structure by the CVD spinning process. The yarn consists of multiple monolayers of CNTs concentrically assembled in seamless tubules along the yarn axis. This layered structure is assembled from CNTs produced in a gas flow from the CVD reaction with a mixed acetone and ethanol carbon source. The development of a water-densification and spinning process allows us to spin the CNT yarn continuously with a yarn length of over several kilometers and a yarn quality close to conventional textile yarns. The CNTyarn can be controlled to be either hollow or monolithic with compacted or detached CNTmonolayers by controlling the spinning process. This layered multifunctional CNT yarns combine superior mechanical properties, electrical conductivities, and surface structures, and have potential applications as structural fibers, composites, woven fabrics, catalyst supports, energy storage materials, artificial tissue, and so on. The fabrication of a CNT yarn by the CVD spinning process relies on the assembly of CNTs in the gas flow by van der Waals interactions. The CNTs assemble in the gas flow when produced in a sufficiently high yield with a high purity such that interaction occurs. Their assembly is, therefore, greatly dependent on the chemistry of the carbon sources. The assembly of CNTs in the gas flow forms a continuous sock-like CNT integrate, which can be mechanically spun out into a CNT yarn. This process was first demonstrated with ethanol as a carbon source and a twisting spinning performed inside the reactor. Recent work reports that a CNT yarn spun from this process possesses ultrahigh strength after densification of the yarn with an acetone vapor. The spinning of multilayered CNT yarns in this work is based on our discovery that CNTs can self-assemble into a multilayered CNT ‘sock’ in the gas flow when a mixture of acetone and ethanol is used as the carbon source. The synthesis was conducted by the injection of the carbon source dispersed with ferrocene and thiophene into a heated gas-flow reactor in flowing hydrogen (Fig. 1a). The CNT layers in the sock, which can be clearly seen in the gas flow, are continuous, concentric, and discrete (Fig. 1b). The CNTsock was initiated from the upper gas flow and produced continuously, traveling downstream with the gases. The assembly of the CNTs is believed to be associated with the interaction of gas molecules, which drive the CNTs towards the outer circumference of the gas flow where they interact mechanically. The formation of the multilayer structure may result from the higher concentration of CNTs in the gas flow because the CNT yield ( 240mg h ) from the mixed carbon source is double that from ethanol alone ( 110mg h ). The layered CNT sock was densified with water after it came out of the reactor. This is realized by connecting a water tank to the end of the CVD reactor (Fig. 1a). The water tank simultaneously encloses the gas-flow system and provides a soft connection between the reactor and air. This configuration allows the CNT assembly to be drawn out continuously from the high-temperature, hydrogen-containing reactor into the open air in a safe and controlled manner. The CNT sock shrinks immediately into a fiber upon arriving at the water surface (Fig. 1c). The fiber is directed around a rotator in the water and is pulled out into air from the other side (Fig. 1d). It is then directed onto the second spool that rotates in acetone for washing and